**HAL Id: hal-00105812**

**https://hal.archives-ouvertes.fr/hal-00105812**

### Submitted on 12 Oct 2006

**HAL** is a multi-disciplinary open access archive for the deposit and dissemination of sci- entific research documents, whether they are pub- lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.

### L’archive ouverte pluridisciplinaire **HAL, est** destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.

**Unconventional motional narrowing in the optical** **spectrum of a semiconductor quantum dot**

### Alice Berthelot, Ivan Favero, Guillaume Cassabois, Christophe Voisin, Claude Delalande, Philippe Roussignol, Robson Ferreira, Jean-Michel Gérard

**To cite this version:**

### Alice Berthelot, Ivan Favero, Guillaume Cassabois, Christophe Voisin, Claude Delalande, et al.. Un-

### conventional motional narrowing in the optical spectrum of a semiconductor quantum dot. Nature

### Physics, Nature Publishing Group, 2006, 2, pp.759. �10.1038/nphys433�. �hal-00105812�

## ccsd-00105812, version 1 - 12 Oct 2006

### quantum dot

A. Berthelot^{1}, I. Favero^{1}, G. Cassabois^{1}^{,∗}, C. Voisin^{1}, C. Delalande^{1}, Ph. Roussignol^{1}, R. Ferreira^{1}and J. M. G´erard^{2}

1Laboratoire Pierre Aigrain, Ecole Normale Sup´erieure, 24 rue Lhomond 75231 Paris Cedex 5, France

2CEA-CNRS-UJF ”Nanophysics and Semiconductors” Laboratory, CEA/DRFMC/SP2M, 17 rue des Martyrs 38054 Grenoble Cedex 9, France

(Dated: October 12, 2006)

Motional narrowing refers to the striking phenomenon where the resonance line of a system cou- pled to a reservoir becomes narrower when increasing the reservoir fluctuation. A textbook example is found in nuclear magnetic resonance, where the fluctuating local magnetic fields created by ran- domly oriented nuclear spins are averaged when the motion of the nuclei is thermally activated.

The existence of a motional narrowing effect in the optical response of semiconductor quantum dots remains so far unexplored. This effect may be important in this instance since the decoherence dynamics is a central issue for the implementation of quantum information processing based on quantum dots. Here we report on the experimental evidence of motional narrowing in the opti- cal spectrum of a semiconductor quantum dot broadened by the spectral diffusion phenomenon.

Surprisingly, motional narrowing is achieved when decreasing incident power or temperature, in contrast with the standard phenomenology observed for nuclear magnetic resonance.

PACS numbers: 78.67.Hc, 78.55.Cr, 05.40.-a

In the seminal work on motional narrowing by Bloem- bergenet al., relaxation effects in nuclear magnetic reso- nance were beautifully explained by taking into account the influence of the thermal motion of the magnetic nu- clei upon the spin-spin interaction [1]. The general treat- ment of relaxation processes for a system interacting with a reservoir was later formulated by Kubo in a stochastic theory that assumes random perturbations of the sys- tem by a fluctuating environment [2]. Depending on the relative magnitude of the spectral modulation ampli- tude and the inverse of the modulation correlation time, the relaxation dynamics is either in theslow modulation limit, where the optical line-shape reflects directly the statistical distribution of the different system energies, or in the fast modulation limit where the fluctuation is smoothed out and the line-shape is motionally narrowed into a Lorentzian profile. The relevance of motional nar- rowing for the description of relaxation phenomena has spread throughout many different fields, such as spin re- laxation in semiconductors [3], vibrational dephasing in molecular physics [4], or phase noise in optical pumping [5].

The optical spectrum of a material system with local- ized, zero-dimensional electronic states provides a generic example of the influence of a fluctuating environment on the coherence relaxation dynamics. In that case, the per- turbing interactions induce a stochastic shift over time of the optical spectrum, resulting in the so-called spectral diffusion effect, which was observed for rare-earth ions [6], molecules [7], or semiconductor quantum dots [8, 9]. In this latter system, impurities, defects or localized charges in the vicinity of a quantum dot induce micro-electric fields that shift the quantum dot emission line through the quantum confined Stark effect. The fluctuation of the quantum dot environment thus randomize the emission energy over a spectral range Σ on a characteristic time

scaleτc. Spectral diffusion under light illumination was reported with jitters of the quantum dot emission energy from hundredsµeV to few meV on time scales ranging from milliseconds to minutes [8, 9, 10]. However, to the best of our knowledge, no evidence for motional narrow- ing (Στc≪~) was pointed out for the spectral diffusion phenomenon in quantum dots.

We present here the experimental evidence for mo- tional narrowing in the optical spectrum of a semicon- ductor quantum dot. High-resolution Fourier-transform spectroscopy performed on the photoluminescence signal of a single InAs/GaAs quantum dot allows the deter- mination of both width and shape of the emission line.

A crossover from Lorentzian to Gaussian profiles of the zero-phonon line is observed while its linewidth increases.

We obtain a quantitative agreement with Monte Carlo simulations where the fluctuating environment is mod- elled by the random capture and escape of carriers in traps located in the quantum dot vicinity. We show that motional narrowing is achieved when decreasing the tem- perature or the incident power because of the asymmetry of the capture and escape mechanisms. Our study pro- vides a counterintuitive example of motional narrowing compared to the standard phenomenology described in nuclear magnetic resonance.

We study self-assembled InAs/GaAs quantum dots grown by molecular beam epitaxy in the Stranski- Krastanow mode, and micro-photoluminescence mea- surements under non-resonant excitation are performed in the far field using the experimental setup described in Ref. [11]. In order to accurately characterize the quan- tum dot emission spectrum, the photoluminescence sig- nal arising from a single quantum dot is analyzed by high-resolution Fourier-transform spectroscopy [11]. The Fourier-transform technique is implemented in the de- tection part of the setup where the photoluminescence

2 signal passes through a Michelson interferometer placed

in front of a 32 cm grating spectrometer. The sig- nal is detected by a low noise Si-based photon count- ing module. With a translation stage, we vary the time t for propagation in one arm of the interferometer and record interferograms of the photoluminescence emission I(t)=I0(1+C(t) cos(E0t/~)), whereI0is the average pho- toluminescence signal intensity,E0 the central detection energy, and C(t) the interference contrast. In the two cases of Lorentzian or Gaussian line-shapes, a Fourier- transform analysis shows that the interference contrast decay is exponential or Gaussian, respectively. As we will see below, the implementation of this technique in single quantum dot spectroscopy allows an accurate de- termination of both width and shape of the emission line.

As far as the linewidth is concerned, sub-µeV measure- ments can be performed by using this interferometric correlation technique [11]. For the determination of the line-shape, our technique allows a high-resolution sam- pling of the Fourier-transform of the spectrum on typi- cally thousands of points. This value is by two orders of magnitude larger than the average number of illuminated pixels in a charge-coupled device in the case of a multi- channel detection in the spectral domain. The drawbacks of our Fourier-transform technique are the long acquisi- tion times of roughly one hour per interferogram, and the required extremely high mechanical stability of the system during the interferogram acquisition.

FIG. 1: Interferogram contrastC(t) of the photoluminescence
signal of a single InAs/GaAs quantum dot at 10K, on semi-
logarithmic plots, for three different incident powers: 0.18
(a), 0.72 (b), and 2.88 kW.cm^{−2} (c). Data (squares), system
response function (dotted line, in red), theoretical fits (solid
line, in green) obtained by the convolution of the system re-
sponse function with Eq. (1), with Στc/~∼0.6 (a), 1.05 (b),
and 1.35 (c), are plotted as a function of the delayt.

In Fig. 1 we display the measured (squares) interfer-
ence contrast C(t) for the emission spectrum of a sin-
gle InAs/GaAs quantum dot at 10K, on semi-logarithmic
plots, for three different incident powers: 0.18 (a), 0.72
(b), and 2.88 kW.cm^{−}^{2} (c). We first observe that the
coherence relaxation dynamics becomes faster when in-
creasing the incident power. Moreover, we notice a grad-
ual modification in the shape of C(t). At low power

(Fig. 1(a)), the interference contrast decay is quasi- exponential with a time constant of 29 ps, thus corre- sponding to a quasi-Lorentzian profile with a full width at half maximum (FWHM) of 45µeV. At higher power (Fig. 1(b)), C(t) has a Gaussian decay at short times (t≤15 ps), and remains exponential at longer times. The line has an intermediate profile, and here its FWHM is 105µeV. At the highest incident power (Fig. 1(c)), the interference contrast decay is predominantly Gaussian, thus corresponding to a quasi-Gaussian profile, with a FWHM of 155µeV.

This crossover from a Lorentzian to a Gaussian line- shape when increasing the incident power reveals an orig- inal relaxation dynamics in semiconductor physics. In fact, in bulk semiconductors or in quantum wells, the standard phenomenology is the exact opposite. An in- creasing number of photo-created carriers leads to the activation of carrier-carrier Coulomb correlations, and induces the inverse transition from an inhomogeneously broadened Gaussian line to a homogeneous Lorentzian one [12]. In the following, we provide a quantitative anal- ysis of our measurements in the framework of the Kubo theory.

Applying the stochastic theory of line-shape and re- laxation of a system coupled to a fluctuating reservoir, the emission spectrum of a quantum dot is conveniently characterized in the time domain and, assuming Gaus- sian fluctuation, the Fourier-transform of the intensity spectrum has the general expression [2]:

C(t) = exp

−Σ^{2}τ_{c}^{2}

~^{2}

exp

−t τc

+ t

τc −1

(1)
In the limit of slow modulation (Στc≫~), the
characteristic function C(t) has a Gaussian decay
(C(t)∼exp(−Σ^{2}t^{2}/2~^{2})): the spectrum reflects directly
the statistical distribution of the emission energies, and
the line-shape is Gaussian with a FWHM given by
2√

2ln2 Σ. In the opposite limit of fast modulation
(Στc≪~), the motional narrowing effect gives rise to an
exponential decoherence (C(t)∼exp(−Σ^{2}τct/~^{2})) with a
decay timeT2=~^{2}/Σ^{2}τc: the fluctuation is smoothed out
by the fast modifications of the reservoir configuration,
and the line-shape becomes Lorentzian with a FWHM
given by 2Σ^{2}τc/~. Indeed, when motional narrowing oc-
curs, the linewidth is reduced by a factor of the order of
Στc/~.

A comparison between our experimental data and the general expression ofC(t) given above allows us to char- acterize the transition from the exponential to the Gaus- sian relaxation observed in Fig. 1. For this purpose, we convolute Eq. (1) with the system response function (dot- ted lines in Fig. 1) which is obtained under white light illumination. The calculated fits are displayed in solid line in Fig. 1. We obtain an excellent agreement with in- creasing values of Στc/~of 0.6 in (a), 1.05 in (b), and 1.35 in (c), where the correlation timeτc has a constant value of 10 ps. The gradual increase of Στc/~ demonstrates the transition from thefast modulation limit to the slow

modulation one when increasing the incident power. As a matter of fact, it shows that motional narrowing oc- curs for low excitation. At first glance, one may think that increasing the number of photo-created carriers in the structure should induce some additional motion in the environment, so that the quantum dot line should be motionally narrowed in the high excitation limit. It is in fact the exact opposite, and we explain below the origin of this unconventional phenomenology.

FIG. 2: (a) Schematic of the quantum dot and its fluctuating
environment: τ_{↓} andτ_{↑} are the capture and escape times of
carriers. (b) Correlation function of the energy fluctuation as
a function of time, on a semi-logarithmic plot: Monte-Carlo
simulations (squares) and exponential fit (solid line). (c) Cor-
relation timeτcnormalized to the capture timeτ_{↓}versusτ_{↓}/τ_{↑}
and (d) spectral modulation amplitude Σ normalized to its
saturation value Σc versus τ_{↓}/τ_{↑}: Monte-Carlo simulations
(squares), and fits (solid lines) according to Eq. (2) for (c)
and Eq. (3) for (d).

The existence of a fluctuating environment around the quantum dot originates from the presence of impurities, defects in the barrier material or in the wetting layer.

Furthermore, this latter heterostructure is far from being an ideal two-dimensional quantum well so that the un- avoidable interface roughness gives also rise to localized states in the quantum dot surroundings [9, 13, 14]. The characteristic parameters Σ and τc are thus determined by the population fluctuation in the various traps located around the quantum dot. We present Monte Carlo sim- ulations of the carrier dynamics in the reservoir for the understanding of the motional narrowing effect in quan- tum dots.

In our model, the fluctuating reservoir consists in N uncorrelated traps which individually induce a Stark shift

∆ of the quantum dot line. This simple scheme has been

chosen for the sake of clarity. More realistic geometries
can be used but do not alter the conclusions. Each trap
is loaded with a characteristic capture timeτ↓, and emp-
tied with an escape time τ↑ (Fig. 2(a)). In our time-
dependent simulations, the random modifications of the
traps population result in fluctuation over timeδE(t) of
the transition energy around a mean value E0. Then,
the spectral modulation amplitude Σ and the correlation
timeτcare calculated by computing the correlation func-
tion of the energy fluctuation X(t), which is defined by
the configuration averageX(t)=hδE(t)δE(0)i [2]. This
correlation function is expected to have an exponential
decay given byX(t)=Σ^{2}exp(−t/τc) [2]. In Fig. 2(b), we
display the correlation functionX(t) computed forN=50
and averaged over one thousand configurations. We ob-
serve on this semi-logarithmic plot the exponential decay
ofX(t), from which we extract Σ andτc. In Fig. 2(c) we
display the correlation timeτc normalized to the capture
timeτ↓as a function of the ratioτ↓/τ↑. We observe that
our calculations are fitted by using the simple expression:

1 τc

= 1 τ↑

+ 1 τ↓

(2) which shows that the correlation time is inversely pro- portional to the total fluctuation rate of the traps popu- lation.

Finally, in Fig. 2(d), we display the spectral modula- tion amplitude Σ normalized to its saturation value Σs. Our numerical simulations are well reproduced by using the expression:

Σ =

√N∆

q_{τ}

↑

τ↓ +q_{τ}

↓

τ↑

(3)

which can also be analytically derived by assuming ergod- icity of the reservoir. The saturation value Σsof the spec- tral modulation amplitude is thus given by√

N∆/2. In semiconductor nanostructures, at low temperature car- rier escape is known to be much less efficient than the capture process [12]. When τ↓/τ↑≪1, the correlation timeτc has approximately a constant value given by τ↓

whereas Σ scales as 2Σs

pτ↓/τ↑. Therefore, an activation of the escape process by raising the incident power will lead to an increase of Στc/~, in qualitative agreement with the phenomenology discussed above.

On the basis of our simple microscopic model, we present a quantitative interpretation of our experiments at 10K as a function of incident power. In Fig. 3 we dis- play the measured values of the FWHM (squares) and Στc/~(circles, inset) as a function of the excitation den- sity, on a semi-logarithmic scale. These two parameters characterize the width of the line-profile and its shape since the crossover from the exponential to the Gaussian decoherence dynamics occurs around Στc/~∼1. We con- front our data with the theoretical values (solid lines) of the FWHM and Στc/~that are calculated with Eq. (1-3), and we observe a fair agreement for the set of parame-

4
ters Σs∼400µeV,τ↓∼10 ps, and 1/τ↑=(1/τ^{0})√

P where
τ0∼1.6 ns andP is in unit of 1 kW.cm^{−}^{2}.

FIG. 3: Full width at half maximum (FWHM) and Στc/~ (inset) of the zero-phonon line of a single quantum dot, at 10K. Data (symbols), and calculations (solid lines) based on Eq. (1-3) are plotted as a function of incident power, on a semi-logarithmic scale.

The asymmetry between the power dependences ofτ↓

andτ↑ stems from the existence of different microscopic processes of various efficiencies in semiconductor physics [12]. The constant value of 10 ps forτ↓is consistent with an optical-phonon assisted capture in the traps around the quantum dot [15]. On the other hand, the inverse process of carrier escape by optical-phonon absorption is strongly inhibited at low temperature, so that it does not significantly contribute to the value of τ↑. In fact, the escape rate dependence on incident power is char- acteristic of Auger-type processes. In the elastic colli- sion of two carriers where one is ejected from the trap while a delocalized carrier relaxes in energy, the escape rate is proportional to the density of delocalized carri- ers, which increases with incident power. In the expres- sion 1/τ↑=(1/τ0)√

P, the sublinear increase of the es- cape rate withP can come from the fact that the actual density of delocalized carriers is governed by bimolecular interband radiative recombination [16] or Auger scatter- ing [17], which both result in a square root dependence of the carrier density on P. Lastly, we note that in the limit of low incident power, the saturation value Σsgiven by√

N∆/2 may be power-dependent due to the reduced number of active traps that are populated from the reser- voir of delocalized carriers. Systematic measurements as a function of temperature and incident power on several quantum dots (to be described elsewhere) allow us to discriminate between the variations of N and τ↑ in our experiments. The power-dependence ofN is found to be negligible in the investigated range of incident power, in agreement with the assumptions made for our calcula- tions.

FIG. 4: (a) Interferogram contrast C(t) of the photolumi-
nescence signal of the quantum dot of Fig. 3 at 35K, for an
incident power of 0.07 kW.cm^{−2}. Data (squares), system re-
sponse function (dotted line, in red), theoretical fit (solid line,
in green) and zero-phonon line contribution (line+empty cir-
cles, in blue) are plotted as a function of the delayt. The
theoretical fit is the convolution of the system response func-
tion with the sum of Eq. (1) with Στc/~

∼ 0.91 (accounting
for the zero-phonon line contribution) and aδ(t)-function (for
the side-bands background). (b) Full width at half maximum
(FWHM) and Στc/~ (inset) of the zero-phonon line of the
quantum dot of Fig. 3, at 0.07 kW.cm^{−2}. Data (symbols),
and calculations (solid lines) based on Eq. (1-3) are plotted
as a function of temperature.

Temperature-dependent experiments performed at low
incident power (0.07 kW.cm^{−2}) reveal the same striking
phenomenology, namely we observe a gradual increase of
Στc/~ with temperature which demonstrates that mo-
tional narrowing occurs at low temperature. However,
the analysis of the data recorded as a function of tem-
perature requires a more careful procedure because the
line-profile exhibits broad side-bands around the central
so-called zero-phonon line [18, 19]. These side-bands are
related to the radiative recombination assisted by the
emission and the absorption of acoustic phonons. At low
temperature (T<25K), their contribution to the total in-
tegrated intensity of the photoluminescence signal is neg-
ligible and can be safely neglected in the data interpreta-
tion, as done for our first set of measurements as a func-
tion of incident power at 10K. Above 25K, the presence
of broad lateral side-bands around the zero-phonon line
results in an interference contrastC(t) with an additional
fast component, the decay of which follows our system re-
sponse function (Fig. 4(a)). By adding a constant term
to the line-profile extracted from Eq. (1), we are able to
fit the whole decay dynamics of the interference contrast
(solid line, in green in (Fig. 4(a)), and thus separate the
relative contributions of the lateral side-bands and zero-
phonon line (line+empty circles, in blue in (Fig. 4(a)).

In Fig. 4(b) we display the measured values of the FWHM (squares) and Στc/~(circles, inset) of the zero- phonon line as a function of the temperature. In the temperature-dependent measurements, the crossover from a Lorentzian to a Gaussian shape of the zero-phonon line occurs when increasing the temperature. More pre- cisely, a smooth transition analog to the one presented in

Fig. 1 is recorded in the temperature range between 30K and 45K. We then confront our data with the theoreti- cal values (solid lines) of the FWHM and Στc/~that are calculated with Eq. (1-3), by assuming that:

1 τ↓

= 1

τ^{1}(1 +n1(T)) + 1

τ^{2}(1 +n2(T)) (4)
1

τ↑

= 1

τ^{1}n^{1}(T) + 1

τ^{2}n^{2}(T) + 1

τ^{3} (5)

In Eq. (5) the constant term inversely proportional to
τ^{3} accounts for the contribution of Auger processes to
carrier escape, as discussed above, and its magnitude is
fixed by the incident power. In the interpretation of our
temperature-dependent measurements, the relevant mi-
croscopic processes for the carrier dynamics in the traps
are phonon-assisted mechanisms where the capture (es-
cape) is thermally-activated due to the emission (absorp-
tion) of an acoustic phonon of mean energy E1 or an
optical phonon of energyE^{2}. The capture and escape ef-
ficiencies are proportional to (1+ni(t)) andni(t) respec-
tively, where ni(t) is a Bose-Einstein occupation factor
given by 1/(exp(Ei/kT)-1). In Fig. 4(b), we observe a
fair agreement between the data and the calculations for
the set of parameters Σs∼400µeV,τ^{1}∼35 ns,τ^{2}∼10 ps,
τ^{3}∼6.5 ns, E^{1}∼1 meV, andE^{2}∼20 meV. This latter ac-
tivation energy is smaller than the characteristic optical
phonon energy of 36 meV in bulk GaAs, and this differ-
ence may come from strain and confinements effects in
the traps formed in the GaAs barrier or in the InAs wet-
ting layer [20]. As far as the carrier dynamics in the traps
is concerned, we find that in our experiments performed
below 50K, the capture process is dominated by optical
phonon emission (τ↓∼τ2). On the other hand, the ther-
mal activation of the escape one is predominantly due
to acoustic phonon absorption below 40K, with an on-
set of optical phonon absorption around 40K. Finally, we
conclude that in the investigated range of temperature,
we are always in the regime where the capture process is
much more efficient than the escape one (τ↓/τ↑≪1), in
exact similarity to the power-dependent experiments at
10K.

The asymmetry of the capture and escape mechanisms
is in fact the fundamental reason why motional narrow-
ing strikingly occurs when decreasing the incident power
or the temperature. If both processes had the same effi-
ciency (τ↑∼τ↓), we would haveτc∼τ↓/2 and Σ∼Σswhich
means that the spectral modulation amplitude would not
depend on the time constant τ↓. Therefore, the ratio
Στc/~could onlydecrease when increasing the reservoir
excitation. This situation corresponds to the well-known
phenomenology from nuclear magnetic resonance where
the activation of the nuclei motion induces the motional
narrowing effect. In the present case whereτ↓/τ↑≤10^{−}^{2},
we are in the opposite regime where the correlation time
is merely constant with relative variation smaller than
10^{−2}whereas the spectral modulation amplitude shows a
steep increase withτ↓/τ↑ (Σ∝p

τ↓/τ↑). The ratio Στc/~ thusincreases when increasing the reservoir excitation.

We conclude that motional narrowing in the optical spectrum of a quantum dot broadened by spectral diffu- sion occurs in the unexpected regime of low temperature and low incident power. This result is of great impor- tance for the applications of quantum dots to quantum information processing. In fact, our study demonstrates that the decoherence dynamics can still be characterized by a decoherence time T2 even in the presence of fluc- tuating local electric fields causing spectral diffusion. In that case, the zero-phonon line has a Lorentzian profile and its width is not given by the intrinsic radiative limit, but by the extrinsic reservoir fluctuation dynamics. In particular, we provide a straightforward interpretation to the widely debated issue of the origin of the temperature dependence of the zero-phonon linewidth. Eventually, we show that the motional narrowing effect strongly re- duces the environment-induced dephasing since the zero- phonon linewidth is approximately Στc/~ smaller than the spectral modulation amplitude 2√

2ln2 Σ due to spec- tral diffusion. This unconventional motional narrowing opens a novel route towards the control of environment- induced dephasing for the applications of quantum dots to quantum information.

∗Electronic address: Guillaume.Cassabois@lpa.ens.fr References

[1] Bloembergen, N., Purcell, E. M. & Pound, R. V. Relax- ation effects in nuclear magnetic resonance, Phys. Rev.

73, 679-715 (1948).

[2] Kubo, R. A stochastic theory of line-shape and relax- ation, inFluctuation, Relaxation and Resonance in Mag- netic Systems(ed D. Ter Haar) 23-68 (Oliver and Boyd, Edinburgh, 1962).

[3] Dyakonov, M. I. & Perel, V. I. Spin orientation of elec- trons associated with the interband absorption of light in semiconductors, Sov. Phys. JETP33, 1053-1059 (1971).

[4] Oxtoby, D. W. Hydrodynamic theory of vibrational de- phasing in liquids, J. Chem. Phys.70, 2605-2610 (1979).

[5] Eberly, J. H., W´odkiewicz, K. & Shore, B. W. Noise

in strong laser-atom interactions: phase telegraph noise, Phys. Rev. A30, 2381-2389 (1984).

[6] Flach, R., Hamilton, D. S., Selzer, P. M. & Yen, W. M.

Time-Resolved Fluorescence Line-Narrowing Studies in
LaF3:Pr^{3+}, Phys. Rev. Lett.35, 1034-1037 (1975).

[7] Ambrose, W. P. & Moerner, W. E. Fluorescence spectroscopy and spectral diffusion of single impurity molecules in a crystal, Nature349, 225-227 (1991).

[8] Empedocles, S. A., Norris, D. J. & Bawendi, M. G. Pho- toluminescence spectroscopy of single CdSe nanocrystal- lite quantum dots, Phys. Rev. Lett.77, 3873-3876 (1996).

[9] Robinson, H. D. & Goldberg, B. B. Light-induced spec- tral diffusion in single self-assembled quantum dots,

6 Phys. Rev. B61, R5086-5089 (2000).

[10] Besombes, L., Kheng, K., Marsal, L. & Mariette, H. Few- particle effects in single CdTe quantum dots, Phys. Rev.

B65, 121314-121317 (2002).

[11] Kammerer, C., Cassabois, G., Voisin, C., Perrin, M., De- lalande, C., Roussignol, Ph. & G´erard, J. M. Interfero- metric correlation spectroscopy in single quantum dots, Appl. Phys. Lett.81, 2737-2739 (2002).

[12] J. Shah, inUltrafast spectroscopy of semiconductors and semiconductor nanostrutures (Spinger-Verlag, Berlin, 1998).

[13] G´erard, J. M., Genin, J. B., Lefebvre, J., Moison, J. M., Lebouche, N. & Barthe, F. Optical investigation of the self-organized growth of InAs/GaAs quantum boxes, J.

Cryst. Growth150, 351-356 (1995).

[14] Heitz, R., Ramachandran, T. R., Kalburge, A., Xie, Q., Mukhametzhanov, I., Chen, P. & Madhukar, A. Obser- vation of reentrant 2D to 3D morphology transition in highly strained epitaxy: InAs on GaAs, Phys. Rev. Lett.

78, 4071-4074 (1997).

[15] Lohner, A., Woerner, M., Elsaesser, M. & Kaiser, W.

Picosecond capture of photoexcited holes by shallow ac- ceptors in p-type GaAs, Phys. Rev. Lett.68, 3920-3923 (1992).

[16] J. E. Carroll, inRate equation in semiconductor electron- ics (Cambridge University Press, 1985).

[17] O’Hara, K. E., Gullingsrud, J. R. & Wolfe, J. P. Auger decay of excitons in Cu2O, Phys. Rev. B60, 10872-10885 (1999).

[18] Besombes, L., Kheng, K., Marsal, L. & Mariette, H.

Acoustic phonon broadening mechanism in single quan- tum dot emission, Phys. Rev. B 63, 155307-155311 (2001).

[19] Favero, I., Cassabois, G., Ferreira, R., Darson, D., Voisin, C., Tignon, J., Delalande, C., Bastard, G., Roussignol, Ph. & G´erard, J. M. Acoustic phonon side-bands in the emission line of single InAs/GaAs quantum dots, Phys.

Rev. B68, 233301-233304 (2003).

[20] Jusserand, B. & Cardona, M., in Light scattering in solids V (eds Cardona, M. & Guntherrodt G.) 49-152 (Springer-Verlag, Heidelberg, 1989).

Acknowledgements

We thank C. Ciuti and B. Gayral for helpful discus- sions. LPA-ENS is ”unit´e mixte (UMR 8551) de l’ENS, du CNRS, des Universit´es Paris 6 et 7”. This work is fi- nancially supported by the region Ile de France through the project SESAME E-1751.

Competing financial interest

The authors declare that they have no competing fi- nancial interests.